text: Testing of CIPP installations is required to confirm that the materials used comply with the site and engineering requirements. Since ground and ambient installation conditions as well as crew skills can affect the success or failure of a cure cycle, testing is performed by 3rd party laboratories in normal cases and should be requested by the owner.
  Samples should be representative of the installation environment since the liner is installed in the ground. Wet sandbags should be used around the restraint where the test sample will be extracted from. As with any specimen preparation for a materials test, it is important to not affect the material properties during the specimen preparation process. Research has shown that test specimen selection can have a significant effect on the CIPP flexural testing results. A technical presentation at the CERIU INFRA 2012 Infrastructures Municipales Conference in Montreal outlined the results of a research project which examined the effects of test specimen preparation on measured flexural properties. Test specimens for ASTM D790 flexural testing must meet the dimensional tolerances of ASTM D790.
  The North American CIPP industry has standardized around the standard ASTM F1216 which uses test specimens oriented parallel with the pipe axis, while Europe uses the standard EN ISO 11296–4 with test specimens oriented in the hoop direction. Research has shown that flexural testing results from the same liner material are usually lower when determined using EN ISO 11296-4 as compared to ASTM F1216.